Three different Ge environments in a new Sr~5~CuGe~9~O~24~ phase synthesized at high pressure and high temperature
Klein, Holger; Kodjikian, Stéphanie; Philippe, Rémy; Ding, Lei; Colin, Claire V.; Darie, Céline; Bordet, Pierre; Acta Crystallographica Section B 76 (2020) 727–732; doi:10.1107/S2052520620008914

data_2108679
_publ_section_title
;
 Three different Ge environments in a new Sr~5~CuGe~9~O~24~ phase
 synthesized at high pressure and high temperature
;
_journal_coeditor_code           JE5030SUP1
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              727
_journal_page_last               732
_journal_paper_doi               10.1107/S2052520620008914
_journal_volume                  76
_journal_year                    2020
_chemical_formula_moiety         'Cu Ge9 O24, 5(Sr)'
_chemical_formula_sum            'Cu Ge9 O24 Sr5'
_chemical_formula_weight         1538.9
_space_group_IT_number           13
_space_group_name_Hall           '-P 2yc'
_space_group_name_H-M_alt        'P 1 2/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 101.5972(13)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   11.8817(3)
_cell_length_b                   8.19277(17)
_cell_length_c                   10.3237(2)
_cell_measurement_temperature    293
_cell_volume                     984.43(4)
_diffrn_ambient_temperature      293
_diffrn_detector                 'linear PSD'
_diffrn_detector_type            Elphyse
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Bruker D5000 diffractometer'
_diffrn_radiation_monochromator  'Ge 111'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a~1~'
_diffrn_radiation_wavelength     1.54056
_diffrn_source                   'sealed X-ray tube'
_diffrn_source_target            Cu
_exptl_absorpt_coefficient_mu    34.454
_exptl_crystal_density_diffrn    5.1917
_exptl_crystal_description       'powder sample'
_exptl_crystal_F_000             488
_pd_meas_2theta_range_inc        0.032
_pd_meas_2theta_range_max        90.317
_pd_meas_2theta_range_min        10.000
_pd_meas_number_of_points        2515
_pd_proc_2theta_range_inc        0.032
_pd_proc_2theta_range_max        90.317
_pd_proc_2theta_range_min        10
_pd_proc_ls_background_function  '19 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_prof_R_factor        0.0284
_pd_proc_ls_prof_wR_expected     0.0243
_pd_proc_ls_prof_wR_factor       0.0376
_refine_diff_density_max         0.60
_refine_diff_density_min         -0.62
_refine_ls_goodness_of_fit_all   1.55
_refine_ls_number_constraints    14
_refine_ls_number_parameters     110
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0276
_refine_ls_R_factor_gt           0.0272
_refine_ls_shift/su_max          0.0240
_refine_ls_shift/su_mean         0.0026
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         0.0299
_refine_ls_wR_factor_gt          0.0299
_cod_data_source_file            je5030sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        984.44(4)
_cod_original_sg_symbol_H-M      'P 2/c'
_cod_database_code               2108679
_publcif_datablock.id            {77930d42-7380-44a8-bc2f-2d2bb7687b21}
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
_publcif_funding_html
;
;